#------------------------------------------------------------------------------
#$Date: 2016-03-23 16:50:47 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179396 $
#$URL: svn://www.crystallography.net/cod/cif/4/32/93/4329326.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4329326
loop_
_publ_author_name
'Xiaowei Ma'
'Banghao Chen'
'Susan E. Latturner'
_publ_contact_author_address
;
 Department of Chemistry and Biochemistry
 Florida State University
 Tallahassee, FL  32306
;
_publ_contact_author_email       latturne@chem.fsu.edu
_publ_contact_author_fax         8506448281
_publ_contact_author_name        'Prof. Susan E. Latturner'
_publ_contact_author_phone       8506444047
_publ_section_title
;
 Synthesis and Properties of New Multinary Silicides R5Mg5Fe4AlxSi18-x (R
 = Gd, Dy, Y, x~ 12) Grown in Mg/Al Flux
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              6089
_journal_page_last               6095
_journal_paper_doi               10.1021/ic202735b
_journal_volume                  51
_journal_year                    2012
_chemical_formula_sum            'Al12 Dy5 Fe4 Mg5 Si6'
_chemical_formula_weight         1649.75
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           123
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   11.655(2)
_cell_length_b                   11.655(2)
_cell_length_c                   4.0668(8)
_cell_measurement_temperature    296(2)
_cell_volume                     552.43(17)
_computing_cell_refinement       'Saint (Bruker, 2008)'
_computing_data_collection       'APEX2 (Bruker, 2008)'
_computing_data_reduction        'Saint (Bruker, 2008)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.951
_diffrn_measured_fraction_theta_max 0.951
_diffrn_measurement_device_type  'Bruker APEX-II CCD area-detector'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0289
_diffrn_reflns_av_sigmaI/netI    0.0123
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -5
_diffrn_reflns_number            6204
_diffrn_reflns_theta_full        28.05
_diffrn_reflns_theta_max         28.05
_diffrn_reflns_theta_min         1.75
_exptl_absorpt_coefficient_mu    20.163
_exptl_absorpt_correction_T_max  0.817
_exptl_absorpt_correction_T_min  0.489
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker, 2008)'
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    4.959
_exptl_crystal_description       rod
_exptl_crystal_F_000             734
_exptl_crystal_size_max          0.04
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.01
_refine_diff_density_max         1.487
_refine_diff_density_min         -0.867
_refine_diff_density_rms         0.201
_refine_ls_extinction_coef       0.0109(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.300
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     35
_refine_ls_number_reflns         428
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.300
_refine_ls_R_factor_all          0.0158
_refine_ls_R_factor_gt           0.0155
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0140P)²+2.1401P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0385
_refine_ls_wR_factor_ref         0.0386
_reflns_number_gt                420
_reflns_number_total             428
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic202735b_si_002_1.cif
_cod_data_source_block           Dy
_cod_original_cell_volume        552.45(18)
_cod_database_code               4329326
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Dy1 Dy 0.26556(3) 0.5000 0.0000 0.00734(14) Uani 1 4 d S
Dy2 Dy 0.0000 0.0000 0.0000 0.01299(19) Uani 1 16 d S
Fe1 Fe 0.29640(9) 0.0000 0.0000 0.0103(2) Uani 1 4 d S
Mg1 Mg 0.20225(15) 0.20225(15) 0.0000 0.0086(5) Uani 1 4 d S
Mg2 Mg 0.5000 0.5000 0.5000 0.0111(10) Uani 1 16 d S
Al1 Al 0.11565(12) 0.37029(13) 0.5000 0.0085(3) Uani 1 2 d S
Al2 Al 0.33148(12) 0.33148(12) 0.5000 0.0030(4) Uani 1 4 d S
Si1 Si 0.17931(18) 0.0000 0.5000 0.0118(4) Uani 1 4 d S
Si2 Si 0.0000 0.5000 0.0000 0.0128(6) Uani 1 8 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Dy Dy -0.1892 4.4098 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Al2 Dy1 Al2 149.59(6) 11_566 1_554
Al2 Dy1 Al2 87.91(3) 11_566 11_565
Al2 Dy1 Al2 84.20(5) 1_554 11_565
Al2 Dy1 Al2 84.20(5) 11_566 .
Al2 Dy1 Al2 87.91(3) 1_554 .
Al2 Dy1 Al2 149.59(6) 11_565 .
Al2 Dy1 Al1 91.13(2) 11_566 .
Al2 Dy1 Al1 106.15(4) 1_554 .
Al2 Dy1 Al1 159.51(5) 11_565 .
Al2 Dy1 Al1 50.28(4) . .
Al2 Dy1 Al1 159.51(5) 11_566 1_554
Al2 Dy1 Al1 50.28(4) 1_554 1_554
Al2 Dy1 Al1 91.13(2) 11_565 1_554
Al2 Dy1 Al1 106.15(4) . 1_554
Al1 Dy1 Al1 82.70(4) . 1_554
Al2 Dy1 Al1 106.15(4) 11_566 13_564
Al2 Dy1 Al1 91.13(2) 1_554 13_564
Al2 Dy1 Al1 50.28(4) 11_565 13_564
Al2 Dy1 Al1 159.51(5) . 13_564
Al1 Dy1 Al1 110.82(5) . 13_564
Al1 Dy1 Al1 58.84(5) 1_554 13_564
Al2 Dy1 Al1 50.28(4) 11_566 13_565
Al2 Dy1 Al1 159.51(5) 1_554 13_565
Al2 Dy1 Al1 106.15(4) 11_565 13_565
Al2 Dy1 Al1 91.13(2) . 13_565
Al1 Dy1 Al1 58.84(5) . 13_565
Al1 Dy1 Al1 110.82(5) 1_554 13_565
Al1 Dy1 Al1 82.70(4) 13_564 13_565
Al2 Dy1 Si2 105.20(3) 11_566 .
Al2 Dy1 Si2 105.20(3) 1_554 .
Al2 Dy1 Si2 105.20(3) 11_565 .
Al2 Dy1 Si2 105.20(3) . .
Al1 Dy1 Si2 55.41(3) . .
Al1 Dy1 Si2 55.41(3) 1_554 .
Al1 Dy1 Si2 55.41(3) 13_564 .
Al1 Dy1 Si2 55.41(3) 13_565 .
Al2 Dy1 Mg2 51.34(4) 11_566 .
Al2 Dy1 Mg2 101.77(2) 1_554 .
Al2 Dy1 Mg2 101.77(2) 11_565 .
Al2 Dy1 Mg2 51.34(4) . .
Al1 Dy1 Mg2 93.50(2) . .
Al1 Dy1 Mg2 148.19(3) 1_554 .
Al1 Dy1 Mg2 148.19(3) 13_564 .
Al1 Dy1 Mg2 93.50(2) 13_565 .
Si2 Dy1 Mg2 143.344(8) . .
Al2 Dy1 Mg2 101.77(2) 11_566 1_554
Al2 Dy1 Mg2 51.34(4) 1_554 1_554
Al2 Dy1 Mg2 51.34(4) 11_565 1_554
Al2 Dy1 Mg2 101.77(2) . 1_554
Al1 Dy1 Mg2 148.19(3) . 1_554
Al1 Dy1 Mg2 93.50(2) 1_554 1_554
Al1 Dy1 Mg2 93.50(2) 13_564 1_554
Al1 Dy1 Mg2 148.19(3) 13_565 1_554
Si2 Dy1 Mg2 143.344(8) . 1_554
Mg2 Dy1 Mg2 73.311(16) . 1_554
Al2 Dy1 Mg1 53.04(3) 11_566 11_565
Al2 Dy1 Mg1 135.26(2) 1_554 11_565
Al2 Dy1 Mg1 53.04(3) 11_565 11_565
Al2 Dy1 Mg1 135.26(2) . 11_565
Al1 Dy1 Mg1 111.25(3) . 11_565
Al1 Dy1 Mg1 111.25(3) 1_554 11_565
Al1 Dy1 Mg1 53.24(3) 13_564 11_565
Al1 Dy1 Mg1 53.24(3) 13_565 11_565
Si2 Dy1 Mg1 78.00(2) . 11_565
Mg2 Dy1 Mg1 99.605(17) . 11_565
Mg2 Dy1 Mg1 99.605(17) 1_554 11_565
Si1 Dy2 Si1 180.00(6) 11 3
Si1 Dy2 Si1 60.90(3) 11 9
Si1 Dy2 Si1 119.10(3) 3 9
Si1 Dy2 Si1 88.43(6) 11 11_556
Si1 Dy2 Si1 91.57(6) 3 11_556
Si1 Dy2 Si1 119.10(3) 9 11_556
Si1 Dy2 Si1 91.57(6) 11 3_554
Si1 Dy2 Si1 88.43(6) 3 3_554
Si1 Dy2 Si1 60.90(3) 9 3_554
Si1 Dy2 Si1 180.00(6) 11_556 3_554
Si1 Dy2 Si1 119.10(3) 11 9_556
Si1 Dy2 Si1 60.90(3) 3 9_556
Si1 Dy2 Si1 88.43(6) 9 9_556
Si1 Dy2 Si1 60.90(3) 11_556 9_556
Si1 Dy2 Si1 119.10(3) 3_554 9_556
Si1 Dy2 Si1 60.90(3) 11 1_554
Si1 Dy2 Si1 119.10(3) 3 1_554
Si1 Dy2 Si1 91.57(6) 9 1_554
Si1 Dy2 Si1 119.10(3) 11_556 1_554
Si1 Dy2 Si1 60.90(3) 3_554 1_554
Si1 Dy2 Si1 180.00(6) 9_556 1_554
Si1 Dy2 Si1 119.10(3) 11 .
Si1 Dy2 Si1 60.90(3) 3 .
Si1 Dy2 Si1 180.0 9 .
Si1 Dy2 Si1 60.90(3) 11_556 .
Si1 Dy2 Si1 119.10(3) 3_554 .
Si1 Dy2 Si1 91.57(6) 9_556 .
Si1 Dy2 Si1 88.43(6) 1_554 .
Si1 Dy2 Mg1 120.451(17) 11 .
Si1 Dy2 Mg1 59.549(17) 3 .
Si1 Dy2 Mg1 120.451(17) 9 .
Si1 Dy2 Mg1 120.451(17) 11_556 .
Si1 Dy2 Mg1 59.549(17) 3_554 .
Si1 Dy2 Mg1 120.451(17) 9_556 .
Si1 Dy2 Mg1 59.549(17) 1_554 .
Si1 Dy2 Mg1 59.549(17) . .
Si1 Dy2 Mg1 59.549(17) 11 9
Si1 Dy2 Mg1 120.451(17) 3 9
Si1 Dy2 Mg1 59.549(17) 9 9
Si1 Dy2 Mg1 59.549(17) 11_556 9
Si1 Dy2 Mg1 120.451(17) 3_554 9
Si1 Dy2 Mg1 59.549(17) 9_556 9
Si1 Dy2 Mg1 120.451(17) 1_554 9
Si1 Dy2 Mg1 120.451(17) . 9
Mg1 Dy2 Mg1 180.00(4) . 9
Si1 Dy2 Mg1 59.549(17) 11 11
Si1 Dy2 Mg1 120.451(17) 3 11
Si1 Dy2 Mg1 120.451(17) 9 11
Si1 Dy2 Mg1 59.549(17) 11_556 11
Si1 Dy2 Mg1 120.451(17) 3_554 11
Si1 Dy2 Mg1 120.451(17) 9_556 11
Si1 Dy2 Mg1 59.549(17) 1_554 11
Si1 Dy2 Mg1 59.549(17) . 11
Mg1 Dy2 Mg1 90.0 . 11
Mg1 Dy2 Mg1 90.0 9 11
Si1 Dy2 Mg1 120.451(17) 11 3
Si1 Dy2 Mg1 59.549(17) 3 3
Si1 Dy2 Mg1 59.549(17) 9 3
Si1 Dy2 Mg1 120.451(17) 11_556 3
Si1 Dy2 Mg1 59.549(17) 3_554 3
Si1 Dy2 Mg1 59.549(17) 9_556 3
Si1 Dy2 Mg1 120.451(17) 1_554 3
Si1 Dy2 Mg1 120.451(17) . 3
Mg1 Dy2 Mg1 90.0 . 3
Mg1 Dy2 Mg1 90.0 9 3
Mg1 Dy2 Mg1 180.00(8) 11 3
Si2 Fe1 Si1 123.87(5) 3_655 .
Si2 Fe1 Si1 123.87(5) 3_655 1_554
Si1 Fe1 Si1 112.26(9) . 1_554
Si2 Fe1 Al1 70.56(4) 3_655 7_556
Si1 Fe1 Al1 62.15(4) . 7_556
Si1 Fe1 Al1 146.94(4) 1_554 7_556
Si2 Fe1 Al1 70.56(4) 3_655 11
Si1 Fe1 Al1 146.94(4) . 11
Si1 Fe1 Al1 62.15(4) 1_554 11
Al1 Fe1 Al1 141.12(8) 7_556 11
Si2 Fe1 Al1 70.56(4) 3_655 11_556
Si1 Fe1 Al1 62.15(4) . 11_556
Si1 Fe1 Al1 146.94(4) 1_554 11_556
Al1 Fe1 Al1 62.80(6) 7_556 11_556
Al1 Fe1 Al1 103.62(6) 11 11_556
Si2 Fe1 Al1 70.56(4) 3_655 7
Si1 Fe1 Al1 146.94(4) . 7
Si1 Fe1 Al1 62.15(4) 1_554 7
Al1 Fe1 Al1 103.62(6) 7_556 7
Al1 Fe1 Al1 62.80(6) 11 7
Al1 Fe1 Al1 141.12(8) 11_556 7
Si2 Fe1 Mg1 114.96(6) 3_655 .
Si1 Fe1 Mg1 76.40(4) . .
Si1 Fe1 Mg1 76.40(4) 1_554 .
Al1 Fe1 Mg1 70.62(4) 7_556 .
Al1 Fe1 Mg1 127.79(3) 11 .
Al1 Fe1 Mg1 127.79(3) 11_556 .
Al1 Fe1 Mg1 70.62(4) 7 .
Si2 Fe1 Mg1 114.96(6) 3_655 11
Si1 Fe1 Mg1 76.40(4) . 11
Si1 Fe1 Mg1 76.40(4) 1_554 11
Al1 Fe1 Mg1 127.79(3) 7_556 11
Al1 Fe1 Mg1 70.62(4) 11 11
Al1 Fe1 Mg1 70.62(4) 11_556 11
Al1 Fe1 Mg1 127.79(3) 7 11
Mg1 Fe1 Mg1 130.07(11) . 11
Si2 Fe1 Dy2 180.0 3_655 .
Si1 Fe1 Dy2 56.13(5) . .
Si1 Fe1 Dy2 56.13(5) 1_554 .
Al1 Fe1 Dy2 109.44(4) 7_556 .
Al1 Fe1 Dy2 109.44(4) 11 .
Al1 Fe1 Dy2 109.44(4) 11_556 .
Al1 Fe1 Dy2 109.44(4) 7 .
Mg1 Fe1 Dy2 65.04(6) . .
Mg1 Fe1 Dy2 65.04(6) 11 .
Fe1 Mg1 Fe1 139.93(11) 3 .
Fe1 Mg1 Al2 104.35(3) 3 .
Fe1 Mg1 Al2 104.35(3) . .
Fe1 Mg1 Al2 104.35(3) 3 1_554
Fe1 Mg1 Al2 104.35(3) . 1_554
Al2 Mg1 Al2 87.34(8) . 1_554
Fe1 Mg1 Al1 137.25(2) 3 7_556
Fe1 Mg1 Al1 54.49(3) . 7_556
Al2 Mg1 Al1 50.93(3) . 7_556
Al2 Mg1 Al1 107.84(7) 1_554 7_556
Fe1 Mg1 Al1 137.25(2) 3 7
Fe1 Mg1 Al1 54.49(3) . 7
Al2 Mg1 Al1 107.84(7) . 7
Al2 Mg1 Al1 50.93(3) 1_554 7
Al1 Mg1 Al1 85.41(4) 7_556 7
Fe1 Mg1 Al1 54.49(3) 3 1_554
Fe1 Mg1 Al1 137.25(2) . 1_554
Al2 Mg1 Al1 107.84(7) . 1_554
Al2 Mg1 Al1 50.93(3) 1_554 1_554
Al1 Mg1 Al1 154.13(10) 7_556 1_554
Al1 Mg1 Al1 88.85(5) 7 1_554
Fe1 Mg1 Al1 54.49(3) 3 .
Fe1 Mg1 Al1 137.25(2) . .
Al2 Mg1 Al1 50.93(3) . .
Al2 Mg1 Al1 107.84(7) 1_554 .
Al1 Mg1 Al1 88.85(5) 7_556 .
Al1 Mg1 Al1 154.13(10) 7 .
Al1 Mg1 Al1 85.41(4) 1_554 .
Fe1 Mg1 Si1 49.62(4) 3 3_554
Fe1 Mg1 Si1 103.94(7) . 3_554
Al2 Mg1 Si1 151.52(4) . 3_554
Al2 Mg1 Si1 88.87(3) 1_554 3_554
Al1 Mg1 Si1 154.87(9) 7_556 3_554
Al1 Mg1 Si1 91.30(3) 7 3_554
Al1 Mg1 Si1 50.25(4) 1_554 3_554
Al1 Mg1 Si1 104.08(4) . 3_554
Fe1 Mg1 Si1 103.94(7) 3 1_554
Fe1 Mg1 Si1 49.62(4) . 1_554
Al2 Mg1 Si1 151.52(4) . 1_554
Al2 Mg1 Si1 88.87(3) 1_554 1_554
Al1 Mg1 Si1 104.08(4) 7_556 1_554
Al1 Mg1 Si1 50.25(4) 7 1_554
Al1 Mg1 Si1 91.30(3) 1_554 1_554
Al1 Mg1 Si1 154.87(9) . 1_554
Si1 Mg1 Si1 56.45(7) 3_554 1_554
Fe1 Mg1 Si1 103.94(7) 3 .
Fe1 Mg1 Si1 49.62(4) . .
Al2 Mg1 Si1 88.87(3) . .
Al2 Mg1 Si1 151.52(4) 1_554 .
Al1 Mg1 Si1 50.25(4) 7_556 .
Al1 Mg1 Si1 104.08(4) 7 .
Al1 Mg1 Si1 154.87(9) 1_554 .
Al1 Mg1 Si1 91.30(3) . .
Si1 Mg1 Si1 107.12(10) 3_554 .
Si1 Mg1 Si1 81.20(5) 1_554 .
Fe1 Mg1 Si1 49.62(4) 3 3
Fe1 Mg1 Si1 103.94(7) . 3
Al2 Mg1 Si1 88.87(3) . 3
Al2 Mg1 Si1 151.52(4) 1_554 3
Al1 Mg1 Si1 91.30(3) 7_556 3
Al1 Mg1 Si1 154.87(9) 7 3
Al1 Mg1 Si1 104.08(4) 1_554 3
Al1 Mg1 Si1 50.25(4) . 3
Si1 Mg1 Si1 81.20(5) 3_554 3
Si1 Mg1 Si1 107.12(10) 1_554 3
Si1 Mg1 Si1 56.45(7) . 3
Al2 Mg2 Al2 90.0 9_666 11_566
Al2 Mg2 Al2 90.0 9_666 3_655
Al2 Mg2 Al2 180.0 11_566 3_655
Al2 Mg2 Al2 180.0 9_666 .
Al2 Mg2 Al2 90.0 11_566 .
Al2 Mg2 Al2 90.0 3_655 .
Al2 Mg2 Dy1 55.440(4) 9_666 11_566
Al2 Mg2 Dy1 55.440(4) 11_566 11_566
Al2 Mg2 Dy1 124.560(4) 3_655 11_566
Al2 Mg2 Dy1 124.560(4) . 11_566
Al2 Mg2 Dy1 55.440(4) 9_666 9_666
Al2 Mg2 Dy1 124.560(4) 11_566 9_666
Al2 Mg2 Dy1 55.440(4) 3_655 9_666
Al2 Mg2 Dy1 124.560(4) . 9_666
Dy1 Mg2 Dy1 69.120(8) 11_566 9_666
Al2 Mg2 Dy1 124.560(4) 9_666 3_655
Al2 Mg2 Dy1 124.560(4) 11_566 3_655
Al2 Mg2 Dy1 55.440(4) 3_655 3_655
Al2 Mg2 Dy1 55.440(4) . 3_655
Dy1 Mg2 Dy1 180.0 11_566 3_655
Dy1 Mg2 Dy1 110.880(8) 9_666 3_655
Al2 Mg2 Dy1 55.440(4) 9_666 9_665
Al2 Mg2 Dy1 124.560(4) 11_566 9_665
Al2 Mg2 Dy1 55.440(4) 3_655 9_665
Al2 Mg2 Dy1 124.560(4) . 9_665
Dy1 Mg2 Dy1 110.880(8) 11_566 9_665
Dy1 Mg2 Dy1 73.312(16) 9_666 9_665
Dy1 Mg2 Dy1 69.120(8) 3_655 9_665
Al2 Mg2 Dy1 55.440(4) 9_666 11_565
Al2 Mg2 Dy1 55.440(4) 11_566 11_565
Al2 Mg2 Dy1 124.560(4) 3_655 11_565
Al2 Mg2 Dy1 124.560(4) . 11_565
Dy1 Mg2 Dy1 73.312(16) 11_566 11_565
Dy1 Mg2 Dy1 110.880(8) 9_666 11_565
Dy1 Mg2 Dy1 106.688(16) 3_655 11_565
Dy1 Mg2 Dy1 69.120(8) 9_665 11_565
Al2 Mg2 Dy1 124.560(4) 9_666 3_656
Al2 Mg2 Dy1 124.560(4) 11_566 3_656
Al2 Mg2 Dy1 55.440(4) 3_655 3_656
Al2 Mg2 Dy1 55.440(4) . 3_656
Dy1 Mg2 Dy1 106.688(16) 11_566 3_656
Dy1 Mg2 Dy1 69.120(8) 9_666 3_656
Dy1 Mg2 Dy1 73.312(16) 3_655 3_656
Dy1 Mg2 Dy1 110.880(8) 9_665 3_656
Dy1 Mg2 Dy1 180.000(6) 11_565 3_656
Al2 Mg2 Dy1 124.560(4) 9_666 1_556
Al2 Mg2 Dy1 55.440(4) 11_566 1_556
Al2 Mg2 Dy1 124.560(4) 3_655 1_556
Al2 Mg2 Dy1 55.440(4) . 1_556
Dy1 Mg2 Dy1 69.120(8) 11_566 1_556
Dy1 Mg2 Dy1 106.688(16) 9_666 1_556
Dy1 Mg2 Dy1 110.880(8) 3_655 1_556
Dy1 Mg2 Dy1 180.0 9_665 1_556
Dy1 Mg2 Dy1 110.880(8) 11_565 1_556
Dy1 Mg2 Dy1 69.120(8) 3_656 1_556
Al2 Mg2 Dy1 124.560(4) 9_666 .
Al2 Mg2 Dy1 55.440(4) 11_566 .
Al2 Mg2 Dy1 124.560(4) 3_655 .
Al2 Mg2 Dy1 55.440(4) . .
Dy1 Mg2 Dy1 110.880(8) 11_566 .
Dy1 Mg2 Dy1 180.0 9_666 .
Dy1 Mg2 Dy1 69.120(8) 3_655 .
Dy1 Mg2 Dy1 106.689(16) 9_665 .
Dy1 Mg2 Dy1 69.120(8) 11_565 .
Dy1 Mg2 Dy1 110.880(8) 3_656 .
Dy1 Mg2 Dy1 73.311(16) 1_556 .
Al2 Al1 Fe1 116.99(4) . 3
Al2 Al1 Fe1 116.99(4) . 3_556
Fe1 Al1 Fe1 103.62(6) 3 3_556
Al2 Al1 Si1 111.00(7) . 3
Fe1 Al1 Si1 56.32(4) 3 3
Fe1 Al1 Si1 56.32(4) 3_556 3
Al2 Al1 Al1 169.81(5) . 5_556
Fe1 Al1 Al1 58.60(3) 3 5_556
Fe1 Al1 Al1 58.60(3) 3_556 5_556
Si1 Al1 Al1 58.80(4) 3 5_556
Al2 Al1 Si2 123.74(4) . 1_556
Fe1 Al1 Si2 119.18(5) 3 1_556
Fe1 Al1 Si2 51.23(3) 3_556 1_556
Si1 Al1 Si2 101.96(4) 3 1_556
Al1 Al1 Si2 61.99(3) 5_556 1_556
Al2 Al1 Si2 123.74(4) . .
Fe1 Al1 Si2 51.23(3) 3 .
Fe1 Al1 Si2 119.18(5) 3_556 .
Si1 Al1 Si2 101.96(4) 3 .
Al1 Al1 Si2 61.99(3) 5_556 .
Si2 Al1 Si2 90.22(4) 1_556 .
Al2 Al1 Mg1 63.45(5) . 1_556
Fe1 Al1 Mg1 119.41(7) 3 1_556
Fe1 Al1 Mg1 54.89(3) 3_556 1_556
Si1 Al1 Mg1 67.39(5) 3 1_556
Al1 Al1 Mg1 109.67(5) 5_556 1_556
Si2 Al1 Mg1 91.243(16) 1_556 1_556
Si2 Al1 Mg1 169.33(7) . 1_556
Al2 Al1 Mg1 63.45(5) . .
Fe1 Al1 Mg1 54.89(3) 3 .
Fe1 Al1 Mg1 119.41(7) 3_556 .
Si1 Al1 Mg1 67.39(5) 3 .
Al1 Al1 Mg1 109.67(5) 5_556 .
Si2 Al1 Mg1 169.33(7) 1_556 .
Si2 Al1 Mg1 91.243(16) . .
Mg1 Al1 Mg1 85.41(4) 1_556 .
Al2 Al1 Dy1 61.85(3) . .
Fe1 Al1 Dy1 86.56(2) 3 .
Fe1 Al1 Dy1 168.10(5) 3_556 .
Si1 Al1 Dy1 135.58(3) 3 .
Al1 Al1 Dy1 124.59(2) 5_556 .
Si2 Al1 Dy1 118.42(5) 1_556 .
Si2 Al1 Dy1 62.60(2) . .
Mg1 Al1 Dy1 125.30(6) 1_556 .
Mg1 Al1 Dy1 71.44(5) . .
Al2 Al1 Dy1 61.85(3) . 1_556
Fe1 Al1 Dy1 168.10(5) 3 1_556
Fe1 Al1 Dy1 86.56(2) 3_556 1_556
Si1 Al1 Dy1 135.58(3) 3 1_556
Al1 Al1 Dy1 124.59(2) 5_556 1_556
Si2 Al1 Dy1 62.60(2) 1_556 1_556
Si2 Al1 Dy1 118.42(5) . 1_556
Mg1 Al1 Dy1 71.44(5) 1_556 1_556
Mg1 Al1 Dy1 125.30(6) . 1_556
Dy1 Al1 Dy1 82.70(4) . 1_556
Al1 Al2 Al1 110.38(9) . 7_556
Al1 Al2 Mg2 124.81(5) . .
Al1 Al2 Mg2 124.81(5) 7_556 .
Al1 Al2 Dy1 134.93(3) . 3_656
Al1 Al2 Dy1 67.87(2) 7_556 3_656
Mg2 Al2 Dy1 73.22(4) . 3_656
Al1 Al2 Dy1 67.87(2) . 1_556
Al1 Al2 Dy1 134.93(3) 7_556 1_556
Mg2 Al2 Dy1 73.22(4) . 1_556
Dy1 Al2 Dy1 82.52(2) 3_656 1_556
Al1 Al2 Dy1 134.93(3) . 3_655
Al1 Al2 Dy1 67.87(2) 7_556 3_655
Mg2 Al2 Dy1 73.22(4) . 3_655
Dy1 Al2 Dy1 87.91(3) 3_656 3_655
Dy1 Al2 Dy1 146.45(7) 1_556 3_655
Al1 Al2 Dy1 67.87(2) . .
Al1 Al2 Dy1 134.93(3) 7_556 .
Mg2 Al2 Dy1 73.22(4) . .
Dy1 Al2 Dy1 146.45(7) 3_656 .
Dy1 Al2 Dy1 87.91(3) 1_556 .
Dy1 Al2 Dy1 82.52(2) 3_655 .
Al1 Al2 Mg1 65.61(4) . 1_556
Al1 Al2 Mg1 65.61(4) 7_556 1_556
Mg2 Al2 Mg1 136.33(4) . 1_556
Dy1 Al2 Mg1 74.31(3) 3_656 1_556
Dy1 Al2 Mg1 74.31(3) 1_556 1_556
Dy1 Al2 Mg1 133.47(4) 3_655 1_556
Dy1 Al2 Mg1 133.47(4) . 1_556
Al1 Al2 Mg1 65.61(4) . .
Al1 Al2 Mg1 65.61(4) 7_556 .
Mg2 Al2 Mg1 136.33(4) . .
Dy1 Al2 Mg1 133.47(4) 3_656 .
Dy1 Al2 Mg1 133.47(4) 1_556 .
Dy1 Al2 Mg1 74.31(3) 3_655 .
Dy1 Al2 Mg1 74.31(3) . .
Mg1 Al2 Mg1 87.34(8) 1_556 .
Fe1 Si1 Fe1 112.26(9) 1_556 .
Fe1 Si1 Al1 61.53(5) 1_556 7_556
Fe1 Si1 Al1 61.53(5) . 7_556
Fe1 Si1 Al1 61.53(5) 1_556 11_556
Fe1 Si1 Al1 61.53(5) . 11_556
Al1 Si1 Al1 62.39(8) 7_556 11_556
Fe1 Si1 Dy2 168.08(7) 1_556 .
Fe1 Si1 Dy2 79.65(3) . .
Al1 Si1 Dy2 127.812(19) 7_556 .
Al1 Si1 Dy2 127.812(19) 11_556 .
Fe1 Si1 Dy2 79.65(3) 1_556 1_556
Fe1 Si1 Dy2 168.08(7) . 1_556
Al1 Si1 Dy2 127.812(19) 7_556 1_556
Al1 Si1 Dy2 127.812(19) 11_556 1_556
Dy2 Si1 Dy2 88.43(6) . 1_556
Fe1 Si1 Mg1 119.52(6) 1_556 .
Fe1 Si1 Mg1 53.982(15) . .
Al1 Si1 Mg1 62.36(5) 7_556 .
Al1 Si1 Mg1 108.52(6) 11_556 .
Dy2 Si1 Mg1 66.89(4) . .
Dy2 Si1 Mg1 121.01(5) 1_556 .
Fe1 Si1 Mg1 53.981(15) 1_556 1_556
Fe1 Si1 Mg1 119.52(6) . 1_556
Al1 Si1 Mg1 62.36(5) 7_556 1_556
Al1 Si1 Mg1 108.52(6) 11_556 1_556
Dy2 Si1 Mg1 121.01(5) . 1_556
Dy2 Si1 Mg1 66.89(4) 1_556 1_556
Mg1 Si1 Mg1 81.20(5) . 1_556
Fe1 Si1 Mg1 119.52(6) 1_556 11
Fe1 Si1 Mg1 53.982(15) . 11
Al1 Si1 Mg1 108.52(6) 7_556 11
Al1 Si1 Mg1 62.36(5) 11_556 11
Dy2 Si1 Mg1 66.89(4) . 11
Dy2 Si1 Mg1 121.01(5) 1_556 11
Mg1 Si1 Mg1 97.95(4) . 11
Mg1 Si1 Mg1 170.18(10) 1_556 11
Fe1 Si1 Mg1 53.981(15) 1_556 11_556
Fe1 Si1 Mg1 119.52(6) . 11_556
Al1 Si1 Mg1 108.52(6) 7_556 11_556
Al1 Si1 Mg1 62.36(5) 11_556 11_556
Dy2 Si1 Mg1 121.01(5) . 11_556
Dy2 Si1 Mg1 66.89(4) 1_556 11_556
Mg1 Si1 Mg1 170.18(10) . 11_556
Mg1 Si1 Mg1 97.95(4) 1_556 11_556
Mg1 Si1 Mg1 81.20(5) 11 11_556
Fe1 Si2 Fe1 180.0 11_565 3
Fe1 Si2 Al1 58.21(3) 11_565 13_565
Fe1 Si2 Al1 121.79(3) 3 13_565
Fe1 Si2 Al1 121.79(3) 11_565 5
Fe1 Si2 Al1 58.21(3) 3 5
Al1 Si2 Al1 180.0 13_565 5
Fe1 Si2 Al1 58.21(3) 11_565 9_566
Fe1 Si2 Al1 121.79(3) 3 9_566
Al1 Si2 Al1 56.02(5) 13_565 9_566
Al1 Si2 Al1 123.98(5) 5 9_566
Fe1 Si2 Al1 121.79(3) 11_565 1_554
Fe1 Si2 Al1 58.21(3) 3 1_554
Al1 Si2 Al1 123.98(5) 13_565 1_554
Al1 Si2 Al1 56.02(5) 5 1_554
Al1 Si2 Al1 180.0 9_566 1_554
Fe1 Si2 Al1 58.21(3) 11_565 9_565
Fe1 Si2 Al1 121.79(3) 3 9_565
Al1 Si2 Al1 116.43(5) 13_565 9_565
Al1 Si2 Al1 63.57(5) 5 9_565
Al1 Si2 Al1 90.22(4) 9_566 9_565
Al1 Si2 Al1 89.78(4) 1_554 9_565
Fe1 Si2 Al1 58.21(3) 11_565 13_564
Fe1 Si2 Al1 121.79(3) 3 13_564
Al1 Si2 Al1 90.22(4) 13_565 13_564
Al1 Si2 Al1 89.78(4) 5 13_564
Al1 Si2 Al1 116.43(5) 9_566 13_564
Al1 Si2 Al1 63.57(5) 1_554 13_564
Al1 Si2 Al1 56.02(5) 9_565 13_564
Fe1 Si2 Al1 121.79(3) 11_565 5_556
Fe1 Si2 Al1 58.21(3) 3 5_556
Al1 Si2 Al1 89.78(4) 13_565 5_556
Al1 Si2 Al1 90.22(4) 5 5_556
Al1 Si2 Al1 63.57(5) 9_566 5_556
Al1 Si2 Al1 116.43(5) 1_554 5_556
Al1 Si2 Al1 123.98(5) 9_565 5_556
Al1 Si2 Al1 180.0 13_564 5_556
Fe1 Si2 Al1 121.79(3) 11_565 .
Fe1 Si2 Al1 58.21(3) 3 .
Al1 Si2 Al1 63.57(5) 13_565 .
Al1 Si2 Al1 116.43(5) 5 .
Al1 Si2 Al1 89.78(4) 9_566 .
Al1 Si2 Al1 90.22(4) 1_554 .
Al1 Si2 Al1 180.0 9_565 .
Al1 Si2 Al1 123.98(5) 13_564 .
Al1 Si2 Al1 56.02(5) 5_556 .
Fe1 Si2 Dy1 90.0 11_565 .
Fe1 Si2 Dy1 90.0 3 .
Al1 Si2 Dy1 61.99(3) 13_565 .
Al1 Si2 Dy1 118.01(3) 5 .
Al1 Si2 Dy1 118.01(3) 9_566 .
Al1 Si2 Dy1 61.99(3) 1_554 .
Al1 Si2 Dy1 118.01(3) 9_565 .
Al1 Si2 Dy1 61.99(3) 13_564 .
Al1 Si2 Dy1 118.01(3) 5_556 .
Al1 Si2 Dy1 61.99(3) . .
Fe1 Si2 Dy1 90.0 11_565 9_565
Fe1 Si2 Dy1 90.0 3 9_565
Al1 Si2 Dy1 118.01(3) 13_565 9_565
Al1 Si2 Dy1 61.99(3) 5 9_565
Al1 Si2 Dy1 61.99(3) 9_566 9_565
Al1 Si2 Dy1 118.01(3) 1_554 9_565
Al1 Si2 Dy1 61.99(3) 9_565 9_565
Al1 Si2 Dy1 118.01(3) 13_564 9_565
Al1 Si2 Dy1 61.99(3) 5_556 9_565
Al1 Si2 Dy1 118.01(3) . 9_565
Dy1 Si2 Dy1 180.0 . 9_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Dy1 Al2 2.9296(7) 11_566
Dy1 Al2 2.9296(7) 1_554
Dy1 Al2 2.9296(7) 11_565
Dy1 Al2 2.9296(7) .
Dy1 Al1 3.0778(12) .
Dy1 Al1 3.0779(12) 1_554
Dy1 Al1 3.0779(12) 13_564
Dy1 Al1 3.0779(12) 13_565
Dy1 Si2 3.0952(7) .
Dy1 Mg2 3.4060(5) .
Dy1 Mg2 3.4060(5) 1_554
Dy1 Mg1 3.548(2) 11_565
Dy2 Si1 2.9159(15) 11
Dy2 Si1 2.9159(15) 3
Dy2 Si1 2.9159(15) 9
Dy2 Si1 2.9159(15) 11_556
Dy2 Si1 2.9159(15) 3_554
Dy2 Si1 2.9159(15) 9_556
Dy2 Si1 2.9159(15) 1_554
Dy2 Si1 2.9159(15) .
Dy2 Mg1 3.334(3) .
Dy2 Mg1 3.334(3) 9
Dy2 Mg1 3.334(3) 11
Dy2 Mg1 3.334(3) 3
Fe1 Si2 2.3729(11) 3_655
Fe1 Si1 2.4490(14) .
Fe1 Si1 2.4490(14) 1_554
Fe1 Al1 2.5871(10) 7_556
Fe1 Al1 2.5871(10) 11
Fe1 Al1 2.5871(10) 11_556
Fe1 Al1 2.5871(10) 7
Fe1 Mg1 2.6002(10) .
Fe1 Mg1 2.6002(10) 11
Mg1 Fe1 2.6002(10) 3
Mg1 Al2 2.945(2) .
Mg1 Al2 2.945(2) 1_554
Mg1 Al1 2.9982(13) 7_556
Mg1 Al1 2.9982(12) 7
Mg1 Al1 2.9982(13) 1_554
Mg1 Al1 2.9982(13) .
Mg1 Si1 3.1245(15) 3_554
Mg1 Si1 3.1245(15) 1_554
Mg1 Si1 3.1245(15) .
Mg1 Si1 3.1245(15) 3
Mg2 Al2 2.778(2) 9_666
Mg2 Al2 2.778(2) 11_566
Mg2 Al2 2.778(2) 3_655
Mg2 Al2 2.778(2) .
Mg2 Dy1 3.4060(5) 11_566
Mg2 Dy1 3.4060(5) 9_666
Mg2 Dy1 3.4060(5) 3_655
Mg2 Dy1 3.4060(5) 9_665
Mg2 Dy1 3.4060(5) 11_565
Mg2 Dy1 3.4060(5) 3_656
Mg2 Dy1 3.4060(5) 1_556
Al1 Al2 2.5559(18) .
Al1 Fe1 2.5871(10) 3
Al1 Fe1 2.5871(10) 3_556
Al1 Si1 2.602(2) 3
Al1 Al1 2.696(3) 5_556
Al1 Si2 2.8701(11) 1_556
Al1 Si2 2.8701(11) .
Al1 Mg1 2.9982(13) 1_556
Al1 Dy1 3.0779(12) 1_556
Al2 Al1 2.5559(18) 7_556
Al2 Dy1 2.9296(7) 3_656
Al2 Dy1 2.9296(7) 1_556
Al2 Dy1 2.9296(7) 3_655
Al2 Mg1 2.945(2) 1_556
Si1 Fe1 2.4489(14) 1_556
Si1 Al1 2.602(2) 7_556
Si1 Al1 2.602(2) 11_556
Si1 Dy2 2.9159(15) 1_556
Si1 Mg1 3.1245(15) 1_556
Si1 Mg1 3.1245(15) 11
Si1 Mg1 3.1245(15) 11_556
Si2 Fe1 2.3730(11) 11_565
Si2 Fe1 2.3730(11) 3
Si2 Al1 2.8701(11) 13_565
Si2 Al1 2.8701(11) 5
Si2 Al1 2.8701(11) 9_566
Si2 Al1 2.8701(11) 1_554
Si2 Al1 2.8701(11) 9_565
Si2 Al1 2.8701(11) 13_564
Si2 Al1 2.8701(11) 5_556
Si2 Dy1 3.0952(7) 9_565
